Direct synthesis of carbon nanofibers from South African coal fly ash
© Hintsho et al.; licensee Springer. 2014
Received: 2 June 2014
Accepted: 1 August 2014
Published: 10 August 2014
Carbon nanofibers (CNFs), cylindrical nanostructures containing graphene, were synthesized directly from South African fly ash (a waste product formed during the combustion of coal). The CNFs (as well as other carbonaceous materials like carbon nanotubes (CNTs)) were produced by the catalytic chemical vapour deposition method (CCVD) in the presence of acetylene gas at temperatures ranging from 400°C to 700°C. The fly ash and its carbonaceous products were characterized by transmission electron microscopy (TEM), thermogravimetric analysis (TGA), laser Raman spectroscopy and Brunauer-Emmett-Teller (BET) surface area measurements. It was observed that as-received fly ash was capable of producing CNFs in high yield by CCVD, starting at a relatively low temperature of 400°C. Laser Raman spectra and TGA thermograms showed that the carbonaceous products which formed were mostly disordered. Small bundles of CNTs and CNFs observed by TEM and energy-dispersive spectroscopy (EDS) showed that the catalyst most likely responsible for CNF formation was iron in the form of cementite; X-ray diffraction (XRD) and Mössbauer spectroscopy confirmed these findings.
KeywordsFly ash Catalytic chemical vapour decomposition Carbon nanofibers Iron
The synthesis of carbon nanomaterials (CNMs) has received tremendous interest in the last two decades [1–5]. These endeavours have been driven by the need to exploit the unique chemical and physical properties associated with CNMs (e.g. strength [6, 7]), as well as the desire to develop synthetic strategies that are cost-effective and non-destructive to the environment [8–10]. The synthesis of well-structured CNMs is known to require three main components: a source of energy, a source of carbon and a template or catalyst . Recent publications have shown that efforts have focused on using lower energy sources (low-temperature synthesis), natural or recyclable carbon reactants and appropriate templates [12–15].
One of the main challenges in the chemical industry has been the development of low-cost, recyclable and effective substrates (catalysts) upon which well-structured CNMs can grow [16–18]. This has prompted interest in several industrial by-products that contain components that are known to actively decompose carbon reagents into CNMs [19–22]. Of interest has been the study of the effect of coal fly ash as a catalyst for carbon nanomaterial growth. Fly ash is typically a by-product of several energy and power generation industries throughout the world, with an estimated 25 million tons produced annually in South Africa . Currently, only a fraction of this material is utilized effectively, with the remainder proving to be environmentally hazardous due to the presence of several toxic elements like mercury, lead, etc. [24–26]. It has been observed that fly ash can be effective at producing carbon nanotubes (CNTs), provided that the reaction conditions are correct (as summarised below) [13, 27, 28]. This is due mainly to the transition metal contents in certain fly ashes. Generally, fly ash consists of SiO2 (c.a. 73.6%), Al2O3 (c.a. 18.7%), Fe2O3 (c.a. 1.9%) and TiO2 (c.a. 1.4%) and can also include trace amounts of CaO, BaO, MgO, MnO, P2O5 as well as copper and chromium oxides . However, metals such as Fe/Ni, Ni, Co, Mn, Cu, V, Cr, Mo and Pd have been used in the past as catalysts for CNT and carbon nanofiber (CNF) syntheses [30–35], hence the potential of fly ash to be used as a catalyst in this reaction. In this regard, Yasui et al.  have used Japanese fly ash, where Fe was added to the ash to enhance its activity. Although CNTs were produced, these were of a very low yield and poor quality. Dunens et al.  showed that CNTs and CNFs could be produced by Australian coal fly ash using the chemical vapour deposition (CVD) method. However, in their case, multiple steps were followed, as iron (which was low in their fly ash, <2.5%) also had to be impregnated into their substrate and ethylene (an expensive carbon source) was used. This therefore resulted in the high cost of CNT and CNF production, although a recycled waste material was used as a catalyst. In an effort to improve the aforementioned processes, Salah et al.  used carbon-rich Saudi Arabian fly ash to produce CNTs. These tubes were also synthesized through a CVD process, but pre-treatment of the ash to remove unburned carbon was required in order to use the ash as a catalyst.
Reports on the effectiveness of fly ash as a catalyst or template in the synthesis of CNFs are limited [27, 28, 36]. Moreover, fly ash is either considered as a support for other more active metallic catalyst particles [28, 36] or used after extensive synthetic treatment . On the other hand, no work has been done using the South African coal fly ash to make CNFs.
This article reports a simple, direct route for the synthesis of CNFs from South African coal fly ash and acetylene at varying temperatures. Here no pre-treatments or additions of expensive catalysts were required, as the fly ash was used as received.
Waste South African coal fly ash was obtained from the Electricity Supply Commission (ESCOM) Research and Innovation Centre (Rosherville, South Africa) and was used without any chemical pre-treatments or thermal modifications. Carbon deposition was achieved by the catalytic chemical vapour deposition method (CCVD) of acetylene over the waste coal fly ash. In these reactions, the coal fly ash was the catalyst, acetylene the carbon source and hydrogen the carrier gas, to create an optimal reaction environment [37–39]. In each synthesis run, 500 mg of as-received fly ash was uniformly spread in a small quartz boat and placed in the centre of a horizontal furnace. The coal fly ash was then heated at 10°C/min in H2 at 100 ml/min to temperatures between 400°C and 700°C in 100°C increments, where upon acetylene gas was introduced into the reaction zone at 100 ml/min for 30 min. After 30 min of reaction time, the flow of acetylene was terminated and the reactor was cooled under H2 to ambient temperature. The resultant carbonaceous material was then harvested for characterization.
The chemical composition of South African coal fly ash samples obtained by XRF
Fly ash component
Particle size distributions were obtained from the TEM micrographs. The particle size distributions of as-received and acetylene-treated coal fly ash (at different temperatures) were also determined using a Malvern particle size analyser (Master Sizer 2000, Malvern Instruments Ltd., Worcestershire, UK). Both these materials were analysed by dispersing them in two different solutions: (1) water and (2) a Dolapix solution (100 ml water:2 ml Dolapix (Zschimmer & Schwarz, Lahnstein, Germany)). Laser Raman spectroscopy was used to ascertain the type of carbonaceous materials that were formed. The thermal stability of the acetylene-treated fly ash products was determined by using a PerkinElmer Pyris 1 thermogravimetric analyser (TGA; PerkinElmer, Waltham, MA, USA). In these measurements, a 10 mg sample was heated to 900°C at a rate of 10°C/min under air (20 ml/min). The specific surface areas of approximately 200 mg of as-received and acetylene-treated fly ash materials (between 400°C and 700°C) were determined using the Brunauer-Emmett-Teller (BET) surface area method by N2 adsorption using an ASAP 2000 Micrometrics Tristar surface area and porosity analyser (Micromeritics Instrument Co., Norcross, GA, USA). Both materials were degassed at 150°C for 4 h under nitrogen before testing to remove the moisture. Mössbauer spectroscopy measurements were carried out in transmission mode with a 10 miC 57Co(Rh) source. Measurements were performed at room temperature on the as-received and acetylene-treated fly ash samples at 700°C.
Results and discussion
For this type of growth to occur, it is known that there is normally a weak interaction between the catalyst and support . During this process, the carbon reagent decomposes on the metal particle under specific reaction conditions. The carbon deposited on the metal then either dissolves/re-precipitates to form either CNT/CNFs, or the carbon migrates over the metal particle to form a tube/fibre . If the catalyst particles are large, then multi-walled carbon nanotubes (MWCNTs) and CNFs may be formed .
Thermogravimetric analyses were carried out to investigate the thermal degradation behaviour of as-received and acetylene-treated fly ash. It has been reported that the graphitic nature of CNMs is directly proportional to their thermal stability . Hence, the first-order weight derivatives of the data so obtained typically gives an indication of the type of carbon present (Figure 4). Typically, highly crystalline nanofibers have been found to be resistant to oxidation when compared to other forms of carbon . Additionally, the diameters and the amount of defects in such materials have also been known to influence their oxidation temperatures . From the TGA thermograms, it was observed that all of the CNMs produced had final oxidation temperatures that were greater than 550°C. However, as previously stated, at least two different forms of carbon were synthesized when the reaction temperature was 500°C. These may have arisen due to the poor carbonization of acetylene, leading to impurities such as amorphous carbon and hence the formation of a higher degree of non-graphitic carbonaceous materials, as confirmed by the laser Raman results (Figure 3a). However, CNFs synthesized at 700°C had the highest oxidation temperature (c.a. 690°C). These results concurred with the laser Raman data, where CNFs formed at 700°C displayed the lowest ID/IG ratio, i.e. they were the most graphitic.
Particle size and surface area measurements
In Figure 6, the materials found in the TEM images of the as-received and acetylene-treated fly ash samples at 500°C were measured. As can be seen, there was a huge reduction in the particle sizes measured by TEM, as compared to when the materials were measured using the particle size analyser (Figure 6). It was noted though that one of the drawbacks of using the particle size analyser was that it did not allow particles to be individually measured. This explains the reduction in size when the data (Figure 6) was compared to the TEM analyses, as particles were individually measured. In the latter case, the average size was found to be 57 and 28 nm for as-received fly ash and CNFs from acetylene-treated coal fly ash, respectively. To confirm these findings, BET was used to study their surface areas (Figure 7). The results showed that the CNFs produced at 500°C displayed the highest surface area (59 m2/g). Studies have shown that the lower the particle size, the higher the surface area .
Composition, mineral phase and oxidation state studies
The major phases in the as-received coal fly ash were quartz (SiO2), hematite (α-Fe2O3) and mullite (3Al2O3 · 2SiO2). After exposure to acetylene, it was noted that peak shifting and broadening had occurred, as was most evident in quartz at 26.5° (2θ). This may have been caused by amorphous glassy phases, found in the as-received fly ash, which when exposed to acetylene and hydrogen became more crystalline . The iron content with the presence of silicates also became more apparent after CNF formation. However, the new phase of iron could not be identified by XRD (which is a bulk technique). Previous studies have shown that when iron is in low quantities and high dispersions, some of its phases cannot be identified using XRD . Likewise for iron, it has been shown that in such cases, the exact phase identification by XRD is difficult as it tends to form a large variety of carbides . In one study, cementite (Fe3C), which could not be identified by XRD, was observed by Mössbauer spectroscopy during the formation of CNTs over iron catalysts from acetylene decomposition . Hence, 57Fe Mössbauer spectroscopy, which is able to identify all forms of iron, was employed in this study. In order to obtain the chemical and structural information of iron-containing materials, three main hyperfine parameters, namely the isomer shift, quadrupole splitting and magnetic splitting, need to be investigated.
Room-temperature Mössbauer parameters for as-received and acetylene-treated coal fly ash samples
After exposure to acetylene, only one sextet, SX1_T, with a reduced magnetic field was observed in the spectrum with hyperfine parameters of Bhf = 20.5 T, δ = 0.29 mm/s; ΔEQ = −0.003 mm/s which has been identified as nanocrystalline iron carbide (Fe3C). The hyperfine parameters of δ = 0.43 mm/s; ΔEQ = 0.41 mm/s and δ = 1.02 mm/s; ΔEQ = 2.15 mm/s obtained for D1_T and D2_T, respectively, were very similar to those obtained for the as-received sample except for the quadrupole splitting of D1_T which was lower and indicated some structural relaxation.
For the as-received fly ash sample, the total population of the oxides was 66% with the remaining fraction of 34% attributed to silicates. After exposure to acetylene, a decrease in the area fraction of 17% was observed for the oxides with a corresponding increase in the silicates. The abundance of the Fe2+ state before treatment was approximately 11% but showed an increase of approximately 19% after acetylene treatment due to the reduced magnetic field.
These results indicate a reduction in the oxidation state of iron (with decreasing oxide content), as a new phase of iron (Fe3C) and silica emerged. This suggestion is in agreement with He et al., who have studied Mössbauer spectroscopy of CNT formation from acetylene which reacted over iron-supported zeolite catalysts and who have found that the +3 oxidation state of iron was reduced to +2 by H2, which they concluded was the active phase for their synthesis . Dunens et al. found that iron also appeared in different forms in their ash and that H2 could not reduce these, presumably because of their location in the fly ash particles . Hence, in their study, unlike in this present work, Dunens et al. were required to further impregnate their ash with iron in order for CNT/CNF growth to occur. In a similar manner, Diamond , using acid etching techniques, demonstrated that the location of the iron and its morphology greatly differed for every fly ash particle within the sample. This, he suggested, was caused by the inhomogeneous nature of coal.
The magnetic feature for the as-received sample was fitted with three sextets (SX1_U, SX2_U and SX3_U) and the spectrum for the acetylene-treated sample was analysed with one sextet (SX1_T), while the non-magnetic spectral components for both samples were fitted with two quadrupole split doublets.
CNFs (and a small amount of CNTs) were successfully produced by directly using an as-received South African coal fly ash. The smooth, glassy and inert surfaces of the South African coal fly ash were covered with irregularly shaped CNFs in the presence of acetylene and hydrogen at temperatures as low as 400°C. Laser Raman spectroscopy confirmed the formation of CNFs. TGA showed that there were different forms of carbon present, i.e. graphitic and amorphous. On the other hand EDS, XRD and Mössbauer spectroscopy confirmed that iron, most likely in the form of iron carbide, was directly associated with the formation of CNFs. Therefore, this study has demonstrated the successful synthesis of carbon nanostructured materials from waste South African coal fly ash without chemical pre-treatments (such as the impregnation of other metals) or thermal modifications. Since CNFs may in the future be beneficial for applications such as particulate nanofillers in polymer matrices, this intervention could result in the reduction of environmental pollutants. Concomitantly, this may also bring relief to the financial burden involved in the disposal costs of this and related coal fly ash around the world in the long run.
NH holds a master's degree and is currently a PhD student at the University of the Witwatersrand. AS received his PhD after publishing in high impact factor journals and is now working at the Registrar's office at the University of the Witwatersrand. PF received his PhD from Cambridge University (UK) and is now working as a lecturer at the University of the Witwatersrand. HM holds a PhD and is a lecturer at the School of Physics. DN holds a PhD and is the head of the Mössbauer facility at the School of Physics. DB holds a PhD, is a professor and is the head of the XRD unit at the Wits School of Chemistry. SD holds a PhD and is currently a senior lecturer and research focus area coordinator for CNTs and strong composites in the DST-NRF Centre of Excellence in Strong Materials at the University of the Witwatersrand.
The authors would like to thank Dr P. Tripathi for his assistance with the artwork in this paper as well as Mr T. Coetzee and Mr M. Khuzwayo who were the initial research assistants in this project. This work is based on the research supported in part by the National Research Foundation of South Africa (Grant Number 88076), ESKOM and the DST-NRF Centre of Excellence in Strong Materials at the University of the Witwatersrand. We are thankful to the Electron and Microscopy Unit (EMU) at the University of the Witwatersrand for TEM analysis.
- White RJ, Luque R, Budarin VL, Clark JH, Macquarrie DJ: Supported metal nanoparticles on porous materials: methods and applications. Chem Soc Rev 2009, 38: 481–494. 10.1039/b802654hView ArticleGoogle Scholar
- Harris PJF: Carbon Nanotube Science: Synthesis, Properties and Applications. Cambridge: Cambridge University Press; 2009:314.View ArticleGoogle Scholar
- Bhaviripudi S, Mile E, Steiner SA, Zare AT, Dresselhaus MS, Belcher AM, Kong J: CVD synthesis of single-walled carbon nanotubes from gold nanoparticle catalysts. J Am Chem Soc 2007, 129: 1516–1517. 10.1021/ja0673332View ArticleGoogle Scholar
- Cantoro M, Hofmann S, Pisana S, Scardaci V, Parvez A, Ducati C, Ferrari AC, Blackburn AM, Wang K-Y, Robertson J: Catalytic chemical vapor deposition of single-wall carbon nanotubes at low temperatures. Nano Lett 2006, 6: 1107–1112. 10.1021/nl060068yView ArticleGoogle Scholar
- Couteau E, Hernadi K, Seo JW, Thien-Nga L, Mikó C, Gaal R, Forro L: CVD synthesis of high-purity multiwalled carbon nanotubes using CaCO3 catalyst support for large-scale production. Chem Phys Lett 2003, 378: 9–17. 10.1016/S0009-2614(03)01218-1View ArticleGoogle Scholar
- Thostenson ET, Ren Z, Chou T-W: Advances in the science and technology of carbon nanotubes and their composites: a review. Compos Sci Technol 2001, 61: 1899–1912. 10.1016/S0266-3538(01)00094-XView ArticleGoogle Scholar
- Wang J: Carbon-nanotube based electrochemical biosensors: a review. Electroanalysis 2005, 17: 7–14. 10.1002/elan.200403113View ArticleGoogle Scholar
- Breuer O, Sundararaj U: Big returns from small fibers: a review of polymer/carbon nanotube composites. Polym Compos 2004, 25: 630–645. 10.1002/pc.20058View ArticleGoogle Scholar
- Callis JB, Illman DL, Kowalski BR: Process analytical chemistry. Anal Chem 1987, 59: 624A-637A.View ArticleGoogle Scholar
- Hutchison JE: Greener nanoscience: a proactive approach to advancing applications and reducing implications of nanotechnology. ACS Nano 2008, 2: 395–402. 10.1021/nn800131jView ArticleGoogle Scholar
- Seah CM, Chai SP, Mohamed AR: Synthesis of aligned carbon nanotubes. Carbon 2011, 49: 4613–4635. 10.1016/j.carbon.2011.06.090View ArticleGoogle Scholar
- Paul KT, Satpathy S, Manna I, Chakraborty K, Nando G: Preparation and characterization of nano structured materials from fly ash: a waste from thermal power stations, by high energy ball milling. Nanoscale Res Lett 2007, 2: 397–404. 10.1007/s11671-007-9074-4View ArticleGoogle Scholar
- Wang S: Application of solid ash based catalysts in heterogeneous catalysis. Environ Sci Tech 2008, 42: 7055–7063. 10.1021/es801312mView ArticleGoogle Scholar
- Shaikjee A, Coville NJ: The role of the hydrocarbon source on the growth of carbon materials. Carbon 2012, 50: 3376–3398. 10.1016/j.carbon.2012.03.024View ArticleGoogle Scholar
- Usubharatana P, McMartin D, Veawab A, Tontiwachwuthikul P: Photocatalytic process for CO2 emission reduction from industrial flue gas streams. Ind Eng Chem Res 2006, 45: 2558–2568. 10.1021/ie0505763View ArticleGoogle Scholar
- Thavasi V, Singh G, Ramakrishna S: Electrospun nanofibers in energy and environmental applications. Energ Environ Sci 2008, 1: 205–221. 10.1039/b809074mView ArticleGoogle Scholar
- Zaera F: The new materials science of catalysis: toward controlling selectivity by designing the structure of the active site. J Phys Chem Lett 2010, 1: 621–627. 10.1021/jz9002586View ArticleGoogle Scholar
- MacKenzie KJ, Dunens OM, Harris AT: An updated review of synthesis parameters and growth mechanisms for carbon nanotubes in fluidized beds. Ind Eng Chem Res 2010, 49: 5323–5338. 10.1021/ie9019787View ArticleGoogle Scholar
- Moravsky AP, Loutfy RO: Double-walled carbon nanotubes and methods for production and application. EP Patent 2010, 1: 328,472.Google Scholar
- Byrappa K: Novel hydrothermal solution routes of advanced high melting nanomaterials processing. J Ceram Soc Jpn 2009, 117: 236–244. 10.2109/jcersj2.117.236View ArticleGoogle Scholar
- Li J, Zhang JZ: Optical properties and applications of hybrid semiconductor nanomaterials. Coord Chem Rev 2009, 253: 3015–3041. 10.1016/j.ccr.2009.07.017View ArticleGoogle Scholar
- Baxter J, Bian Z, Chen G, Danielson D, Dresselhaus MS, Fedorov AG, Fisher TS, Jones CW, Maginn E, Kortshagen U: Nanoscale design to enable the revolution in renewable energy. Energ Environ Sci 2009, 2: 559–588. 10.1039/b821698cView ArticleGoogle Scholar
- Minchener AJ: Coal gasification for advanced power generation. Fuel 2005, 84: 2222–2235. 10.1016/j.fuel.2005.08.035View ArticleGoogle Scholar
- Ferraiolo G, Zilli M, Converti A: Fly ash disposal and utilization. J Chem Technol Biotechnol 1990, 47: 281–305.View ArticleGoogle Scholar
- Gupta UC, Gupta SC: Trace element toxicity relationships to crop production and livestock and human health: implications for management. Comm Soil Sci Plant Anal 1998, 29: 1491–1522. 10.1080/00103629809370045View ArticleGoogle Scholar
- Finkelman RB, Belkin HE, Centeno JA: Health impacts of coal: should we be concerned? Geotimes 2006, 51: 24.Google Scholar
- Salah N, Habib SS, Khan ZH, Memic A, Nahas MN: Growth of carbon nanotubes on catalysts obtained from carbon rich fly ash. Digest Journal of Nanomaterials and Biostructures 2012, 7: 1279–1288.Google Scholar
- Yasui A, Kamiya Y, Sugiyama S, Ono S, Noda H, Ichikawa Y: Synthesis of carbon nanotubes on fly ashes by chemical vapor deposition processing. IEEJ Trans Electr Electron Eng 2009, 4: 787–789. 10.1002/tee.20481View ArticleGoogle Scholar
- Nath DC, Sahajwalla V: Application of fly ash as a catalyst for synthesis of carbon nanotube ribbons. J Hazard Mater 2011, 192: 691–697. 10.1016/j.jhazmat.2011.05.072View ArticleGoogle Scholar
- Li Y, Li D, Wang G: Methane decomposition to COx-free hydrogen and nano-carbon material on group 8–10 base metal catalysts: a review. Catal Today 2011, 162: 1–48. 10.1016/j.cattod.2010.12.042View ArticleGoogle Scholar
- Huczko A: Template-based synthesis of nanomaterials. Applied Physics A 2000, 70: 365–376. 10.1007/s003390051050View ArticleGoogle Scholar
- Terrones M, Hsu WK, Kroto HW, Walton DR: Nanotubes: a revolution in materials science and electronics. In Fullerenes and Related Structures. Heidelberg: Springer; 1999:189–234.View ArticleGoogle Scholar
- Rummeli MH, Schäffel F, Bachmatiuk A, Adebimpe D, Trotter G, Borrnert F, Scott A, Coric E, Sparing M, Rellinghaus B: Investigating the outskirts of Fe and Co catalyst particles in alumina-supported catalytic CVD carbon nanotube growth. ACS Nano 2010, 4: 1146–1152. 10.1021/nn9016108View ArticleGoogle Scholar
- Lai C, Guo Q, Wu X-F, Reneker DH, Hou H: Growth of carbon nanostructures on carbonized electrospun nanofibers with palladium nanoparticles. Nanotechnology 2008, 19: 195303. 10.1088/0957-4484/19/19/195303View ArticleGoogle Scholar
- Bing Y, Liu H, Zhang L, Ghosh D, Zhang J: Nanostructured Pt-alloy electrocatalysts for PEM fuel cell oxygen reduction reaction. Chem Soc Rev 2010, 39: 2184–2202. 10.1039/b912552cView ArticleGoogle Scholar
- Dunens OM, MacKenzie KJ, Harris AT: Synthesis of multiwalled carbon nanotubes on fly ash derived catalysts. Environ Sci Tech 2009, 43: 7889–7894. 10.1021/es901779cView ArticleGoogle Scholar
- Yu Z, Chen D, Tøtdal B, Holmen A: Parametric study of carbon nanofiber growth by catalytic ethylene decomposition on hydrotalcite derived catalysts. Mater Chem Phys 2005, 92: 71–81. 10.1016/j.matchemphys.2004.12.032View ArticleGoogle Scholar
- Melechko AV, Merkulov VI, McKnight TE, Guillorn M, Klein KL, Lowndes DH, Simpson ML: Vertically aligned carbon nanofibers and related structures: controlled synthesis and directed assembly. J Appl Phys 2005, 97: 041301–041301–041339.View ArticleGoogle Scholar
- Plata DL, Meshot ER, Reddy CM, Hart AJ, Gschwend PM: Multiple alkynes react with ethylene to enhance carbon nanotube synthesis, suggesting a polymerization-like formation mechanism. ACS Nano 2010, 4: 7185–7192. 10.1021/nn101842gView ArticleGoogle Scholar
- Fenelonov V, Mel'gunov M, Parmon V: The properties of cenospheres and the mechanism of their formation during high-temperature coal combustion at thermal power plans. KONA Powder and Particle Journal 2010, 28: 189–207. 10.14356/kona.2010017View ArticleGoogle Scholar
- Coville NJ, Mhlanga SD, Nxumalo EN, Shaikjee A: A review of shaped carbon nanomaterials. S Afr J Sci 2011, 107: 01–15.View ArticleGoogle Scholar
- Gong QM, Li Z, Wang Y, Wu B, Zhang Z, Liang J: The effect of high-temperature annealing on the structure and electrical properties of well-aligned carbon nanotubes. Mater Res Bull 2007, 42: 474–481. 10.1016/j.materresbull.2006.06.023View ArticleGoogle Scholar
- Shanahan PV, Xu L, Liang C, Waje M, Dai S, Yan Y: Graphitic mesoporous carbon as a durable fuel cell catalyst support. J Power Sources 2008, 185: 423–427. 10.1016/j.jpowsour.2008.06.041View ArticleGoogle Scholar
- Lehman JH, Terrones M, Mansfield E, Hurst KE, Meunier V: Evaluating the characteristics of multiwall carbon nanotubes. Carbon 2011, 49: 2581–2602. 10.1016/j.carbon.2011.03.028View ArticleGoogle Scholar
- Teng F, Ting J-M, Sharma SP, Liao K-H: Growth of CNTs on Fe–Si catalyst prepared on Si and Al coated Si substrates. Nanotechnology 2008, 19: 095607. 10.1088/0957-4484/19/9/095607View ArticleGoogle Scholar
- Bartolome JF, De Aza AH, Martin A, Pastor JY, Llorca J, Torrecillas R, Bruno G: Alumina/zirconia micro/nanocomposites: a new material for biomedical applications with superior sliding wear resistance. J Am Ceram Soc 2007, 90: 3177–3184. 10.1111/j.1551-2916.2007.01884.xView ArticleGoogle Scholar
- Pérez-Cabero M, Taboada J, Guerrero-Ruiz A, Overweg A, Rodríguez-Ramos I: The role of alpha-iron and cementite phases in the growing mechanism of carbon nanotubes: a 57Fe Mössbauer spectroscopy study. Phys Chem Chem Phys 2006, 8: 1230–1235. 10.1039/b516243bView ArticleGoogle Scholar
- He N, Kuang Y, Dai Q, Miao Y, Zhang A, Wang X, Song K, Lu Z, Yuan C: Growth of carbon nanotubules on Fe-loading zeolites and investigation of catalytic active center. Mater Sci Eng C 1999, 8: 151–157.View ArticleGoogle Scholar
- Diamond S: Particle morphologies in fly ash. Cem Concr Res 1986, 16: 569–579. 10.1016/0008-8846(86)90095-5View ArticleGoogle Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/4.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly credited.